7 G. Conte1**, P. Allegrini1, M. Pacilli1, S. Salvatori2, D.M. Trucchi3, T. Kononenko4,5,
A. Bolshakov4,5, V. Ralchenko4,5, V. Konov4,5
1University Roma Tre, Dept of Sciences, Rome, Italy 2University Niccolò Cusano, Rome, Italy 3Material Science Institute, Monterotondo Scalo, Italy 4A.M. Prokhorov General Physics Institute, Moscow, Russia 5National Research Nuclear University “MEPhI”, Moscow, Russia
Abstract. The charge collection performance of a diamond-graphite detector is reported. Buried graphite pillars
with high aspect ratio were formed inside a single crystal synthetic diamond slab by using a femtosecond IR laser with 200 kHz of repetition rate. Grouped in two series and connected by graphite strips on the surface, eight independent 3D electrodes were used to collect the charge carriers generated by energy deposited in the detector. Collimated 90Sr,Y -particles were used to test the charge collection in coincidence and self-triggering mode among pillars rows using different irradiation geometries. The charge collected by one pillar row saturates at 1.40±0.02fC at ±0.67V/m with electrons impinging orthogonally the rows demonstrating a high charge carrier collection efficiency.
Key words:CVD Diamond, Electric contacts, Graphite pillars, 3D sensors, -particles
* The paper was presented at the Third International Conference on Radiation and Applications in Various Fields of Research (RAD 2015), Budva, Montenegro, 2015.
** email@example.com 1.INTRODUCTION
Solid carbon shows very different mechanical properties depending on 3D or 2D carbon-carbon bond organization. The first case leads to crystalline diamond with a very tight lattice and the highest mechanical hardness; the latter refers to graphite with ordered planes able to slide one respect the other and leading to lubricant properties. Moreover, considering the high energy needed to displace a single atom from the very compact lattice (1.76×1023 at/cm3), diamond shows also important
electronic properties for the fabrication of devices suitable to detect electromagnetic radiation from UV to the X-ray region  and for charge particles detection in high luminosity/high energy physics experiments . Besides, its wide band gap energy (5.47 eV) makes this solid transparent to VIS-IR radiation also assuring very low electrical conductivity in the dark (<10-15 S/cm). High
mobility (up to 2400 cm2/Vs) and saturation
velocity (∼2×107 cm/s) jointly with charge carriers
lifetimes as high as 0.321 s for electrons and 0.983
s for holes have been demonstrated  in synthetic diamond samples deposited by CVD techniques. The very high thermal conductivity of single crystal diamond (22 W/cm K), concurrently with mechanical and electronic features, ensures power dissipation, temperature stability, charge collection efficiency, high signal sensitivity, fast
transient response, possibility of real-time analysis, low noise and radiation hardness for diamond based devices. All such characteristics are fundamental for radiation detectors suitable to monitor intense pulsed sources like UV lasers, synchrotron radiation beams and X-ray facilities. Detection and tracking of nuclear particles also require sensitive and fast detectors with low electronic noise, assured in this case by the small dielectric permittivity (~5.5) of diamond material. The other ordinate solid form of carbon, the graphite, thanks to its high electrical conductivity (~1.3×103
8 thermal stress and volume expansion. Here we
present a radiation detector with buried graphite pillars having a high aspect ratio, wired among them using surface graphite runners and without the need of more metallic pads. This 3D detector has been simulated, electrically characterized and tested with low activity radioactive sources demonstrating to be suitable for X-rays and electron spectroscopy.
2.EXPERIMENTAL ISSUES 2.1. Material
A single crystal CVD diamond produced by Elements Six, 3×3 mm2 large and 0.5 mm thick was
used in this work. The four lateral faces were lapped using common polishing techniques for further real time observation of the appearance and propagation of laser graphitized regions in the bulk of diamond. A 20x microscope objective and a CCD camera were used for this purpose.
2.2. Graphitization and device realization The diamond sample was installed on a computer-controlled XYZ translation stage equipped with DC motors for precise 3D movement of the focal point regarding the sample surface. Local graphitization of the plate was performed with 400 fs pulses of VaryDisc50 laser (Dausinger+Giesen Gmbh) operated at 1030 nm wavelength at 200 kHz of pulse repetition rate. The laser beam was tightly focused inside the diamond plate and moved in XYZ directions to form conductive graphitic electrodes on the back surface and in the bulk. The pulse energy was varied in the 0.2-0.8 µJ range. Figure 1 shows a graphite pillar 20 m in diameter.
Figure 1. Graphite pillar of 20 m in diameter.
Altogether, 212 parallel buried graphite pillars, 380±20 µm long (deep) and 150±5 µm apart, were produced one by one, with the pillar diameter of about 20 µm (see figure 1). They were grouped in two series along one direction by means of proper planar back contact patterns (~50 μm wide and ~10 μm thick, 150±5 μm apart) realized with the same laser technique. The resulting contacts constitute the terminals for eight different strips (named channels in the following) used for signal acquisition surrounded by others connected pillars used for channel biasing. Due to the pillars planar body centered structure, also considering the wideness of each graphite strip and pillars diameter, in the following we will consider an effective distance among surface strips equal to Leff=120±5 m and
√2Leff m between a couple of isolated pillars
connected to different voltages.
The Raman spectra taken at the strip surface and pillar termination, on the external surface, is a proof of nano-graphite formation. The observed features in the spectra (D and G peaks) were similar to those reported elsewhere for diamond irradiated with a Ti:sapphire laser (1 ps, λ=800 nm). The fabricated device was then glued with silver paste on a double face printed circuit board (PCB) and the first series of pillars wire bonded with 25 m Al/Si standard wires directly on the graphite strips and used as powered electrode. As the formed nano-graphite shows very good adhesion to the underneath diamond, there was the possibility to directly bond the wires. This electrode is located all-around the residual series of connected pillars. The second series forms eight groups of vertical electrodes, 300 m apart, wire bonded separately - without any metallization - to copper strips on the PCB (see figure 2) which are connected to the signal input of a CAEN A1422H-F2 (45 mV/MeV in Si) hybrid charge sensitive amplifier having an input test (C=1pF) to be used for calibration.
Figure 2. 8-Channels wire bonded 3D detector.
9 2.3. Measuring methods
The pulses amplitude distribution and charge carriers collection of each the eight pillars group (a channel) was analyzed under collimated 1 MBq
90Sr,Y test source, 1 mm in diameter (QSA Global,
code SIFB13505, item 22/2006). The source holder and collimator was a brass cylinder 25 mm long, suitable to host the source, with an aperture 0.4 mm in diameter and 5 mm deep on one side, located at different distance from the detector depending on the test. Two different measurement setups were used: (i) fast counting collection in self triggering mode on each digitizer channel; (ii) slow counting collection mode using the smallest selectable coincidence window, equal to 10 ns, between two collecting channels among the eight available ones. High voltage CAEN N1471A power supply and two different digitizers: CAEN N6724A 2-cannels, 14 bit, 100 MS/s and 500 mVpp of dynamic range was used
for data collection and spectroscopy analysis using CAEN DPP-PHA digital pulse processing package; V1724 8-channels, 14 bit, 100 MS/s and 500 mVpp
for traces dumping - 10s of acquisition time - using the N6724A coincidence output trigger. An Agilent 33250A waveform generator with suitable rise and decay built-in curves was used to produce a calibration curve to convert the pulse height distribution in the ADC channels to equivalent electrons and collected charge. The calibration curve was linear with slope b=2.66 aC/ADC channel and constant parameter a=16.3 aC.
3.RESULTS AND DISCUSSION
3.1. Current-Voltage characteristic
The current versus voltage I(V) curve, in the dark, up to ±100V of channel-n.8 is reported in figure 3. A Keithley 6517A picoammeter was used for this purpose at room temperature and with zero current correction. Before the measurement, aimed to remove possible adsorbed water from the surface, the device was heated at 250 °C in air for 300 s.
10-12 10-11 10-10 10-9
1 10 100
Graphite Pillars Channel n.8
Absolute Voltage (V) Ohmic trend
Figure 3. Channel n.8 Current vs Voltage I(V) characteristic.
Figure 4. Electric field 3D analysis of a buried graphite pillars detector. The picture shows a zoomed region deep inside the bulk diamond. Blue color indicates high electric field.
3.2. Response to 90Sr,Y -particles
Initially, aimed to evaluate the eight channels collection features, the signal dependence on voltage was measured in self-triggering mode on all channels at parallel (vertical) incidence with respect to the pillars row showing their homogeneous response at constant voltage with the source aligned to the channel.
8Ch_Pillars 100V, 1h
y = m1*exp(-(x-m2)^ 2/m3^ 2) Error Value
332,5 5795,9 m1
0,083274 5,2265 m2
0,11777 1,7776 m3
NA 1,1497e+6 Chisq
NA 0,98686 R
y = m1*exp(-(x-m2)^ 2/m3^ 2) Error Value
142,83 9485 m1
0,016197 4,4225 m2
0,023357 1,3303 m3
NA 1,5637e+5 Chisq
NA 0,99921 R
2 4 6 8 10
1 2 3 4 5 6 7 8
Figure 5. Integral number of events measured by the eight channels, monitored two at a time with the source aligned as indicates the inset.
With the source 1 cm apart the detector surface and aligned between Ch4 and Ch5, the integral number of events (green curve) acquired by each channel is reported in figure 5. The number of events follows a Gaussian distribution centered between Ch4 and Ch5. Two more dummy channels, having no counts, have been added. In the same figure it is also reported the integral number of events with an
impinging angle of 10° with respect the vertical direction (red curve). It is worth to note that, as the distribution changes, the maximum decreases in value and shifts to channel position 5.3 whereas the FWHM increases towards an equivalent value of three channels. This result addresses the possibility to use this detector for angle resolved measurements.
0 50 100 150
0 1 2 3 4 5
Collected Charge (fC)
8Ch_Pillars 80V, 2h
Figure 6. Pulse height distribution of central Ch4 and Ch5 at 80V with the orthogonal setup.
The pulse height distributions at 80V of Ch4 and Ch5 are reported in figure 6. Measurements were taken using the internal digitizer self triggering configuration with a voltage threshold fixed to 0.3 mV (12 ADC Channels). The signal monitored for one hour shows an asymmetric distribution with a long exponential decay tail. For the collected charge, the two curves show a most probable value (MPV) equal to 1.75±0.02 fC (about 11000 equivalent electrons), and a FWHM of the distribution of 0.92±0.02 fC.
90Sr,Y radioactive source produces electrons having a
continuous energy - decay spectrum. 90Sr decays by - emission to 90Y with an end-point energy 0.53 MeV,
then new - decay to 90Zr is observed with an
11 “classical” 2D planar capacitor-like architecture: in
other words, it is reasonable expected a poor charge collection efficiency. If we consider, for the sake of simplicity, a high charge collection distance in this single crystal diamond plate, we could consider to collect the charge along the 380 m of average thickness and inside the whole volume among pillars, even if with unknown efficiency. The measured distribution MPV at 1.75±0.02 fC and the average collected charge value <Q>=1.85±0.02 fC indicate a promising result for the implemented detector geometry and demonstrate once again that graphite pillars buried in single-crystal diamond are suitable 3D electrodes for detecting β-particles with high charge collection efficiency.
Besides this study, the response at orthogonal incidence with the source 2 cm apart the pillars row was tested. Figure 7 shows the signal dependence on the collected charge for positive voltages of channel n.8, the nearest to the source and about 0.4 m from the impinging face. The spectrum is mainly due to low-energy electrons penetrating no more than 0.5
0 20 40 60 80 100
0 1 2 3 4 5
8Ch-Graphite Pillars Lateral Incidence, 1h
5V 10V 20V 40V 60V
Collected Charge (fC)
Figure 7. Channel n.8 signal dependence on positive voltage at orthogonal incidence.
The signal increases with voltage and charge collection saturation is observed at 1.38±0.02 fC (8625e) around 80V while the integral number of events increases. The signal dependence on collected charge for negative applied bias is reported in figure 8. Before performing such measurements, the detector was biased at 0.0V for 24 hours in the dark. The digitizer configuration parameters, as voltage threshold, pole-zero cancellation and gain, were not changed with the exception of reversing the signal input. The distribution again saturates around -80V, with a collected charge of 1.40±0.02 fC (8750e). More parameters of curves in figure 7 and 8 are reported in Table 1 for comparison. If we assume the collection volume be defined by the effective distance between two biased pillar’s rows at 250 m, we should expect a release of 9000 equivalent
electron charge (~1.44 fC). This estimation remains, also in this case, very rough because the body centered pillars organization does not give the possibility to exactly define the active collection volume also assuming the charge carriers diffusion.
0 20 40 60 80 100
0 1 2 3 4 5
8Ch-Graphite Pillars Lateral Incidence, 1h
Collected Charge (fC)
Sr 1.4 fC
Figure 8. Channel n.8 signal dependence on negative voltage. The scheme illustrates the incidence geometry.
The small number of total measured events in one hour of acquisition, mainly due to the small collimator aperture, determines a very low signal-to-noise digital ratio; nevertheless, the average collected charge value of 1.39±0.02 fC changing the bias polarity compares very well to the proposed estimation of 1.44 fC and indicates once again a promising situation for this 3D detector and impinging particles geometry for tracking.
Table 1. Relevant parameters of Figure 7-8.
(V) MPV (fC) Counts Peak FWHM (fC)
-80 1.40 70 1.00
-60 1.39 50 0.90
-40 1.35 33 0.83
-20 1.32 14 0.80
-10 1.25 4 0.65
-5 1.12 2 -
5 1.10 2 -
10 1.18 7 0.64
20 1.16 15 0.76
40 1.20 34 0.83
60 1.37 54 0.90
80 1.38 78 1.00
12 was used to activate V1724 digitized and dump 1000
points with 10 ns of resolution of the residual Ch2-7 channels traces. The normalized pulse amplitude distribution measured in coincidence mode by N6724A digitizer is reported in figure 9.
0 0,5 1 1,5
0 1 2 3 4 5
8-Ch. Graphite Pillars Ch.1-8 Coincidence 10 ns Time Window
Collected Charge (fC)
Figure 9. Coincidence pulse height distribution of Ch8 and Ch1.
An acquisition rate of 10 events/h has been evaluated on the two weeks of observation time. It has to be observed that the graphite pillars of Ch8 and Ch1 are about 2.1 mm apart. Notwithstanding the wide coincidence window, for the sake of discussion, there is the possibility to believe the spectrum associated at the energy deposited by the same electron traversing the whole distance between Ch8 and Ch1. On the basis of this hypothesis, we have to find corresponding transitions on the other channels Ch2-7 channels for each coincidence event.
8200 8300 8400 8500 8600 8700
0 2 4 6 8 10
Ch4 Ch5 Ch6
Ch-7 0.73 mV
Figure 10. V1724 traces corresponding at Channel n.2 trough 7 acquired in coincidence with Channel n.1 and n.8.
For instance, figure 10 reports one of such coincidence dump related to channels 2-7 connected
to the V1724 digitizer. Each of the six measured channel has a different offset for better trace visibility. As it is apparent, a step around 1 s is visible on each channel at the same time demonstrating the coincidence among the eight graphite pillars channels. The step amplitude has been evaluated at 0.73±0.06 mV (24±2 ADC channels) with acceptable S/N ratio. To understand the meaning of the showed step, it is worth noting that a 27.8 mV reference pulse sent to the charge sensitive amplifier (CTest=1pF) by the
Agilent 33250A waveform generator produces a step 420±10 ADC channel wide. Thus, showed pulse roughly corresponds to one event around 1.7 fC.
The high efficiency of charge collection revealed in this study agrees with the results reported for other 3D diamond-based detectors fabricated by using femtosecond pulsed laser [6,7]. On the contrary, the detectors of similar geometry produced with nanosecond pulses [7,13] demonstrate significantly lower charge collection efficiency. The opposite tendency is found, however, for electrical conductivity of the graphitized wires: usage of nanosecond pulses provides higher conductivity by one order of magnitude comparing with femtosecond pulses (see, for instance, ). Raman spectroscopy is the only technique applied up to now to investigate composition and internal structure of the graphitized region in the diamond bulk. It reveals some important features like strong mechanical stresses (up to 10 GPa) in the surrounding diamond or intensive fluctuations of graphite concentration over the wire’s length and diameter [7,14], however, these findings don’t explain the mentioned trends in electronic properties. It is noted  that full diamond-graphite transformation inside diamond bulk is impossible due to expected rise of the material compression over the limits, where such transformation is permitted by the thermodynamics. This means that the so-called “graphitized” region unambiguously contains both sp2
and sp3 carbon phases. However, we still have no
information how the irradiation parameters influence relative concentration of both phases and their fracturing. The same relates also to the nature and generation mechanisms of electronic active defects. A further works is required to clarify those issues important for optimizing the detectors structures.
1. M. Girolami, P. Allegrini, G. Conte, S. Salvatori, D.M. Trucchi and V. Ralchenko, “Diamond Detectors for UV and X-Ray Source Imaging,” IEEE-EDL, vol. 33, no.2, pp. 224-226, Feb. 2012.
2. W. Adams et al. (The RD42 Collaboration), “Radiation Hard Diamond Sensors for Future Tracking Applications,” Nucl. Inst. Meth. Phys. Res., vol. A565, no.1, pp. 278–283, June 2006.
3. M. Pomorski et al., “Development of Single-Crystal CVD-Diamond Detectors for Spectroscopy and Timing,” Phys. Stat. Sol. (A), vol. 203, no. 12, pp. 3152–3160, Dec. 2006.
4. M. Pacilli et al., “Beta Particles Sensitivity of an All-Carbon Detector,” Nucl. Inst. Meth. Phys. Res., vol. A738, pp. 119-125, Feb. 2014.
5. A. Oh, B. Caylar, M. Pomorski and T. Wengler, “A Novel Detector with Graphitic Electrodes in CVD Diamond,” Diamond Relat. Mater., vol. 38, pp.9– 13, 2013.
6. T. Kononenko et al., “All-Carbon Detector with Buried Graphite Pillars in CVD Diamond,” Appl. Phys., vol. A114, pp. 297-300, Nov, 2013.
7. S. Lagomarsino et al., “Three-Dimensional Diamond Detectors: Charge Collection Efficiency of Graphitic Electrodes,” Appl. Phys. Lett., vol. 103, pp. 233507-10, Feb. 2013.
8. T.V. Kononenko,V.I. Konov,S.M. Pimenov,N.M. Ros-sukanyi, A.I. Rukovishnikov and V. Romano, “Three-Dimensional Laser Writing in Diamond Bulk,” Diamond Relat. Mater., vol. 20, pp. 264-268, Jan. 2011.
9. V.P. Popov, L.N. Safronova, O.V. Naumova, D.V. Ni- kolaev, I.N. Kupriyanov and Yu.N. Palyanov, “Con-ductive Layers in Diamond Formed by Hydrogen Ion Implantation and Annealing”, Nucl. Inst. Meth. Phys. Res., vol. B282, pp. 100–107, Jan. 2012.
10. F. Picollo et al., “Fabrication and Electrical Characterization of Three-Dimensional Graphitic Microchannels in Single Crystal Diamond,” New Jour. Phys., vol. 14, pp. 053011-20, May 2012.
11. B. Sun, P.S. Salter and M.J. Booth, “High Conductivity Micro-Wires in Diamond Following Arbitrary Paths,” Appl. Phys. Lett., vol.105, pp. 231105 (1-4), Dec. 2014. 12. S. Zhao, “Characterization of the Electrical Properties
of Polycrystalline Diamond Films,” Ph.D. dissertation, Dept. Phys., Ohio State Univ., Columbus, USA, 1994. 13. B. Caylar, M. Pomorski and P. Bergonzo,
“Laser-Processed Three Dimensional Graphitic Electrodes for Diamond Radiation Detectors”, Appl. Phys. Lett., vol.103, pp.043504 (1-3), July 2013.
14. S. Lagomarsino et al., “Electrical and Raman-Imaging Characterization of Laser-Made Electrodes for 3D Diamond Detectors”, Diamond Relat. Mat., vol. 43, pp.23-28, Mar. 2014.